Article
Multiscale Modelling of Hydrogen Transport andSegregation in Polycrystalline Steels
Claas Hüter 1,2,3,∗, Pratheek Shanthraj 1, Eunan McEniry 1, Robert Spatschek 1,2,3 ID ,Tilmann Hickel 1, Ali Tehranchi 1, Xiaofei Guo 4 and Franz Roters 1
1 Max-Planck-Institut für Eisenforschung, Max-Planck-Straße 1, 40237 Düsseldorf, Germany;[email protected] (P.S.); [email protected] (E.M.); [email protected] (R.S.);[email protected] (T.H.); [email protected] (A.T.); [email protected] (F.R.)
2 Institute for Energy and Climate Research, Forschungszentrum Jülich, 52425 Jülich, Germany3 Jülich-Aachen Research Alliance (JARA Energy), RWTH Aachen University, 52056 Aachen, Germany4 Steel Institute, RWTH Aachen University, 52072 Aachen, Germany; [email protected]* Correspondence: [email protected]; Tel.: +49-2461-61-1569
Received: 30 April 2018; Accepted: 4 June 2018; Published: 7 June 2018�����������������
Abstract: A key issue in understanding and effectively managing hydrogen embrittlement incomplex alloys is identifying and exploiting the critical role of the various defects involved.A chemo-mechanical model for hydrogen diffusion is developed taking into account stress gradientsin the material, as well as microstructural trapping sites such as grain boundaries and dislocations.In particular, the energetic parameters used in this coupled approach are determined from ab initiocalculations. Complementary experimental investigations that are presented show that a numericalapproach capable of massive scale-bridging up to the macroscale is required. Due to the wide rangeof length scales accounted for, we apply homogenisation schemes for the hydrogen concentrationto reach simulation dimensions comparable to metallurgical process scales. Via a representativevolume element approach, an ab initio based scale bridging description of dislocation-inducedhydrogen aggregation is easily accessible. When we extend the representative volume approachto also include an analytical approximation for the ab initio based description of grain boundaries,we find conceptual limitations that hinder a quantitative comparison to experimental data in thecurrent stage. Based on this understanding, the development of improved strategies for furtherefficient scale bridging approaches is foreseen.
Keywords: hydrogen embrittlement; multi-scale; multiscale modelling; chemo-mechanics
1. Introduction
Hydrogen embrittlement (HE) can be defined as the structural degradation of materials resultingfrom exposure to hydrogen and often leading to abrupt and premature failure [1–7]. HE in complexengineering materials is increasingly commonplace in key application areas, such as hydrogen-basedenergy conversion cycles [8,9], high strength materials synthesis and coatings [10], marine and deepsea technology as well as structural components in the oil and gas industries [11]. While there is acritical need for such technologies to meet increasing worldwide energy demands, the damage risksassociated with HE has become a substantial bottleneck for further development.
Despite considerable effort, the mechanistic causes for HE are not yet completely understoodowing to its complex nature [12–14]. The competition of different defects for aggregating hydrogen,especially between dislocations and grain boundaries, poses a crucial as well as intricate subjectof investigation in hydrogen embrittlement. Especially for dislocations and grain boundaries,the competitive picture is complemented by possibly cooperative damage facilitation, as hydrogen
Metals 2018, 8, 430; doi:10.3390/met8060430 www.mdpi.com/journal/metals
http://www.mdpi.com/journal/metalshttp://www.mdpi.comhttps://orcid.org/0000-0002-0087-677Xhttp://www.mdpi.com/2075-4701/8/6/430?type=check_update&version=1http://dx.doi.org/10.3390/met8060430http://www.mdpi.com/journal/metals
Metals 2018, 8, 430 2 of 16
transport to grain boundaries via slip transfer. Currently, some viable mechanisms proposed in theliterature are: (i) hydrogen enhanced de-cohesion (HEDE), (ii) hydrogen enhanced localized plasticity(HELP), (iii) hydride-induced embrittlement, and (iv) hydrogen induced super-abundant vacancy(HISAV) formation. In the HEDE mechanism, hydrogen diffusion to and its subsequent interactionwith the strained atomic bonds at the crack tip, result in a lowering of the cohesive energy of thematerial [15], thus making it easier to form a Griffith crack [16–18]. The HELP mechanism wasproposed to account for observations of localized plasticity at the crack tip in a range of metallicsystems [2,19]. It is based on the influence of hydrogen in reducing the mobility of dislocationsby screening their interaction stress fields [20,21]. The corresponding increase in plasticity is highlylocalized owing to the heterogeneous hydrogen distribution due to stress concentrations in the material,and thus culminates prematurely in ductile fracture.
These failure mechanisms and failure-inducing effects depend on localised chemistry, stress anddeformation state, and the defects accessible to damage initiation. We therefore aim at the developmentof an efficient, massively scale-bridging approach that allows for catching process-relevant states ofsteel products, including massive deformations, high defect densities and varying chemical loadings.The approach of choice is a coupled crystal plasticity finite element (CPFEM) phase field model that isimplemented in the Düsseldorf Advanced Material Simulation Kit (DAMASK) [22]. It operates on themacroscale and therefore employs representative volume element (RVE) descriptions that allow forincluding electronic and atomistic scale information about the system via efficient averaging in termsof composite models.
The manuscript is organised as follows: in Section 2, our recent experimental findings in ferriticsteels, which exhibit grain boundary related hydrogen embrittlement, are presented. Hereby, wemotivate the subsequent theoretical considerations. In Section 3, the continuum model is introduced,followed by a brief description of the implementation and the ab initio-based parametrisation.In Section 4, the analytic ab initio based approximations for the influence of dislocations on hydrogenaggregation are introduced and we compare the analytic composite model and the fully numericallyresolved full-field simulation results. Based on the excellent agreement, we extend the compositemodel by an efficient, ab initio based description of grain boundaries. We recognise the conceptualdifficulties to include grain boundaries in terms of a composite model in an RVE spirit. Finally,in Section 5, we summarise the insights gained and relate them to potential future approaches to theinherently massively scale bridging problem of hydrogen embrittlement.
2. Experimental Findings
Our theoretical considerations are complemented by experimental measurements of hydrogen-charged martensitic steel samples, focusing on fracture strength and hydrogen saturation. As weare interested in a qualitative estimate for the difference in hydrogen concentration in steel due todefects relative to a basic Sievert’s law estimate, a cold rolled martensitic stainless steel X20Cr13 ischosen. Here, we expect a high dislocation density and a pronounced effect of defect-mediatedhydrogen aggregation.
Figure 1 shows an example of hydrogen induced cracking in a cold rolled martensitic stainlesssteel X20Cr13 with the chemical composition 0.2% C and 13% Cr in weight percent. The material waspre-charged with hydrogen in 0.05 M H2SO4 and 1.4 g/L Thiourea at the overpotential of −800 mVSCEfrom 0–24 h to bring in different amounts of hydrogen into the material. Hydrogen charging wascarried out with potentiostat High-Power 96 from Bank GmbH, Pohlheim, Germany . A Calomelelectrode was used as a reference electrode and a platinum net was used as the counter electrode.Before charging, the specimen surfaces were ground sequentially from #320 to #800 SiC grit paperand finally polished with 6 µm diamond paste on canvas. After charging, the material was storedin liquid N2 before hydrogen measurement by hot extraction with the hydrogen analysis equipmentLECO RH402. Figure 1a shows the evolution of hydrogen contents according to the charging period.It reveals the material obtained as high as 27 ppm hydrogen after 24 h hydrogen charging. According
Metals 2018, 8, 430 3 of 16
to the Sievert’s law, the solid solubility of hydrogen in pure iron under hydrogen pressure of 100 bar atroom temperature accounts for 2 × 10−7, which is extremely low compared to the amount of hydrogenmeasured in this experiment [23]. Therefore, it is assumed the oversaturated hydrogen due to thehydrogen charging is associated with hydrogen at dislocations and grain boundaries. Figure 1a alsoreveals the sharp reduction of fracture strength due to the charged hydrogen after a slow strain ratetest at the strain rate of 10−6 s−1, which is reduced from 1046 MPa to 432 MPa when the amount ofhydrogen is raised from 1.5 ppm to 20 ppm. Slow strain rate tests were performed with a constantextension machine from Zwick, Ulm, Germany, with a maximum load of 30 kN. The tensile specimensare in dog-bone shape with the geometry A25. Figure 1b illustrates the fracture surface from the failedslow strain rate specimens. The as delivered X20Cr13 has the initial hydrogen content of 1.5 ppm,which exhibits fully ductile (D) fracture feature with very fine dimple sizes. After charging with 5 ppmhydrogen, the fracture surface changes to mixed transgranular (TG) and intergranular (IG) cleavageand a few ductile islands. The cracks are propagating through the prior austenite grain boundariesas well as the martensite lath. By further increasing the charged hydrogen, the TG and IG fracturesbecome more prominent. In association with the sharp reduction in fracture strength, the high amountof charged hydrogen is assumed to be accumulating at the prior austenite grain boundaries andreduces the grain boundary cohesion force.
Figure 1. Hydrogen induced cracking in a cold rolled X20Cr13 martensitic stainless steel. (a) theevolution of hydrogen contents according to the hydrogen charging time and the fracture strengthaccording to the hydrogen charging time determined by a slow strain rate test at the strain rateof 10−6 s−1; (b) fracture surfaces from the failed slow strain rate specimens with different amounts ofpre-charged hydrogen.
The complexity of the possible interpretation of the reported observations suggests a theoreticalapproach that reaches the experimental dimensions. On the other hand, it also needs to catchessential aspects of atomistic and electronic interaction of the hydrogen with the dominant species,here presumably dislocations and grain boundaries. In the following section, the ab initio informedcrystal plasticity model is introduced, which we extend to include the effective description of thesedefect species in the context of hydrogen aggregation.
3. Model Formulation
The description of the entire model covers several aspects on multiple length scales. For anextended discussion of the model, see [24]. Following the continuum picture of the crystal plasticitymodel and hydrogen transport, the numerical implementation is briefly introduced. Based on thecontinuum picture, we explain which insights and parameters from the quantum mechanical level weuse for the scale-bridging approach, and briefly discuss the ab initio model.
Metals 2018, 8, 430 4 of 16
3.1. Continuum Model Formulation
Let B0 ⊂ R3 be a microstructural domain of interest, with boundary ∂B0. The deformationresulting from an applied loading defines a field, χ(x) : x ∈ B0 → y ∈ B, mapping points x in thereference configuration B0 to points y in the deformed configuration B and a concentration field,cH(x) : x ∈ B0 → [0, 1], of the fraction of interstitial lattice positions occupied by hydrogen. The totalfree energy density of this system is composed of mechanical, chemical and gradient contributions:
ftotal = fmech + fchem + fgrad. (1)
The constitutive model for the mechanical free energy density is presented first. Here, the totaldeformation gradient, F = grad χ, is multiplicatively decomposed into an elastic, chemical interstitialand plastic component as
F = FeFiFp. (2)
The elastic deformation gradient, Fe, determines the stress at a material point, where an anisotropicelastic stiffness, C, relates the elastic GREEN–LAGRANGE strain measure [25], E, to the secondPIOLA–KIRCHHOFF stress measure, S [25]:
E =12(Fe
TFe − I), and S = CE. (3)
The chemical deformation gradient, Fi, is determined from the hydrogen concentration, cH,
Fi = eHcHI (4)
and results from the interstitial volumetric change associated with solute hydrogen occupancy, eH.As we explain in more detail in Section 3.2, the concentration field cH will be evaluated basedon different equilibrium approximations. These distinguish whether no defects, dislocations ordislocations and grain boundaries are present in the system. The plastic deformation gradient evolvesaccording to the flow rule
Ḟp = LpFp, (5)
where the plastic velocity gradient, Lp, is driven by the stress through the plasticity model. The crystalplasticity model used in the present study, is an adoption of the phenomenological description ofPeirce et al. [26] for face-centered cubic crystals. The plastic velocity gradient Lp is composed of theslip rates γ̇α on each of the 12 BCC {1 1 0}〈1 1 1〉 slip systems, which are indexed by α = 1, . . . , 12.
Lp = ∑α
γ̇α bα ⊗ nα, (6)
where bα and nα are unit vectors along the slip direction and slip plane normal, respectively. The sliprates are given by
γ̇α = γ̇0
∣∣∣∣ταgα∣∣∣∣n sgn (τα) (7)
in terms of the resolved shear stress, τα = S · (bα ⊗ nα). The slip resistances on each slip system, gα,evolve asymptotically towards g∞ with shear γβ (β = 1, . . . , 12) according to the relationship
ġα = γ̇β h0∣∣∣1− gβ/g∞∣∣∣a sgn(1− gβ/g∞) hαβ (8)
with parameters h0 and a. The interaction between different slip systems is captured by the hardeningmatrix hαβ.
Metals 2018, 8, 430 5 of 16
The constitutive model represents an implicit system of equations to be solved for a consistentelastic and plastic deformation gradient (for details see [27]). The mechanical free energy density isthen given by
fmech =12
S · E (9)
and its minimization results in mechanical equilibrium in terms of the first Piola–Kirchhoff stressmeasure, P,
δ fmechδχ
= Div P = 0. (10)
The chemical free energy density for this system is based on the regular solution model
fchem =1Ω
[EHcH + kBT[cH ln cH + (1− cH) ln(1− cH)]
], (11)
where Ω is the atomic volume, kB is the BOLTZMANN constant, T is the temperature and EH isa hydrogen enthalpy. Though EH belongs to bulk Fe, the development of the hydrogen energydescription given in the subsequent part of this publication will also include dislocations and grainboundaries.
Following [28], the free energy of the interface is given by
fgrad = κ|Grad cH|2, (12)
where κ is the surface energy parameter associated with the diffuse pore–matrix interface.The evolution of the conserved concentration field is then given by the modified Cahn–Hilliard equation
˙cH = Grad ·MH Grad µH, (13)
where MH is the mobility of the hydrogen solute. Their chemical potential µH is thermodynamicallydetermined from the free energy density
µH =δ ftotalδcH
=δ fmech
δcH+
EHΩ
+kBTΩ
ln(
cH1− cH
), (14)
where the mechanical coupling with µH is obtained through Equation (4).
3.2. Numerical Implementation of the Continuum Model
For the numerical implementation of the chemoelastoplastic model, the Düsseldorf AdvancedMaterial Simulation Kit (DAMASK) [22] is used, an open source crystal plasticity finite element library.For the sake of simplicity, we exemplarily introduce here representative volume elements (RVEs) usedfor simulations of fcc materials. The respective numerical parameters will be described correspondinglyin the results part.
RVEs belong to the group of statistical approaches to achieve a representative homogenizationof a material’s microstructure for a macroscopic model. For plasticity models, the varying quantitytypically is the dislocation density. In Figure 2, an example of the RVE for a dislocation density ofρ = 1× 1015 m−2 is shown. The dislocation density ρ is given as ρ = Nd/V, where N is the numberof dislocations, d the circumference of the dislocation line, modeled as ellipse, and V the volume ofthe simulation box. The semi major-axis is labelled a, the semi minor-axis b. The dimensions of thedislocation lines are a = 15 nm± 3 nm and b = 7 nm± 3 nm, where ±3 nm here means that, for eachindividual dislocation line, a value from the interval (−3 : 3) is randomly added to the correspondingbasic value of a and b. The dislocations are equally distributed on all 12 slip systems, i.e., on all12 slip planes, only one dislocation is initially set, and the two additional dislocations are randomly
Metals 2018, 8, 430 6 of 16
distributed to a slip system. These dislocations are randomly positioned on the corresponding slipsystems. Such an RVE thus includes 25 different microstructural phases, i.e., 12 phases enclosed by thedislocations, the 12 dislocations and the matrix phase.
Figure 2. Here, the inner of a dislocation and the dislocation line are shown separately.top: the microstructure index 2–13 refers to the inner of dislocations, bottom: the microstructureindex 14–25 refers to dislocation loops. Microstructure index 1 refers to the matrix and is not shown.
3.3. Atomistic Parameterisation
A key aim of the present work has been to determine the parameters of the continuum modelfrom atomistic simulation. One important parameter is the effective binding energy of H in the vicinityof a dislocation. Evaluating such a binding energy is challenging for a number of reasons. Firstly,the long-range strain field around an ideal straight-line dislocation leads to the requirement of largesimulation cells to avoid elastic artifacts. Moreover, care must be taken to avoid interactions betweenthe interstitial H and its periodic images in the direction of the dislocation line. A third issue is that alarge number of possible configurations must be considered in order to obtain reliable sampling of thepotential energy surfce for hydrogen around such a dislocation.
In order to solve these issues, we utilise the environmental tight-binding (ETB) approach [29,30],which enables the rapid evaluation of energies and forces for systems of arbitrary chemistry, within aquantum-mechanical framework. The current approach requires the full eigenvalue spectrum of aone-electron Hamiltonian matrix, thus solving the one-electron Schrödinger equation within a localatomic-orbital basis set. Due to the cubic scaling of the eigenvalue problem, the present implementationis limited to systems of the order of 103 atoms. The reliability of the approach for the Fe-H system hasbeen demonstrated by examining the H segregation behaviour at a selection of grain boundaries inα-Fe [30].
Metals 2018, 8, 430 7 of 16
The chosen dislocation is the a/2〈111〉 screw dislocation in α-Fe, the behaviour of which ishighly relevant for plastic deformation of iron at low temperatures. In order to circumvent theproblem of long-range strain fields around a dislocation, and to avoid electronic surface effects arisingfrom the application of elastic boundary conditions, the well-known quadrupole construction [31] isused, which allows for the study of dislocations within a periodic cell. In this approach, sketchedschematically in Figure 3, a periodic arrangement of dislocations of opposite Burgers vectors ismade, such that the long-range strain field is eliminated. One must take care that the distancebetween dislocation pairs is sufficiently large so that their mutual interaction (which is of courselong-ranged) does not overshadow the effect under scrutiny. In these simulations, a rectangulararrangement of periodic dislocations is chosen, which allows for the computationally convenient useof an orthorhombic unit cell in the simulations; we found that a cell of 672 atoms is necessary to avoidsignificant augmentation of the core structures of the dislocations.
[112]
[110]
[111]
_
__
Figure 3. Schematic images of the quadrupole dislocation construction used in the simulation. The bluearrows indicate the helicity of the dislocations, with “up” and “down” arrows corresponding to screwdislocations of Burgers vectors b = a/2〈111〉 and −b, respectively. The red circles indicate the effectivebinding range.
Having obtained the relaxed dislocation configuration, the next stage is to assess the bindingenergy of hydrogen to this dislocation. In order to avoid interactions between H atoms and theirperiodic images, the simulation cell is extended by doubling the number of atomic planes along thedirection of the Burgers vector, thus resulting in a H-free simulation cell of 1344 atoms. By numericalsimulation, we find that the dislocation has an effective binding range of ∼5 Å from the centre of thecore. Within this radius, 72 plausible interstitial sites for H are found (per Burgers vector), and thebinding energy of each of these is evaluated (see Figure 4). The maximum value of the binding energy(with respect to a single H atom in a tetrahedral site in bulk α-Fe) is found to be 0.34 eV at the core ofthe dislocation. The median value of the binding energies is Ēbind = 0.14 eV, for a core radius rc = 5 Å.To account for the entropic contribution of the dislocations, Ēbind is shifted by kBT ln(Vdislocation/Vvoxel)in the scale bridging simulations.
Metals 2018, 8, 430 8 of 16
-0.4 -0.2 0 0.2 0.4 0.6Energy (eV)
0
1
2
3
4
5
6
DO
S (
stat
es/e
V)
Inner Region
Intermediate Region
Outer Region
Density of States
Figure 4. Each vertical line corresponds to one data point (due to symmetry, some points overlap).The colors correspond to the distances from the dislocation core, measured by the radius R. The redcircles correspond to the 24 points closest to the dislocation core (R < 2.87 Å), the green squares are inthe “intermediate range” (2.87 Å < R < 4.04 Å), with the blue points belong are the outermost 24 points.The density of states (DOS) curve is generated by broadening the delta functions by a Lorentzianfunction of width kBT/2 (T = 300 K), with the integral under the DOS curve being normalised to 1.
While it would be possible to resolve the detailed picture presented in Figure 4 on a continuumlevel when we stick to small simulation volumina or low defect complexities, see the resultsreported [20,21], reaching process-relevant simulation boxes in the CPFEM approach requires furtherhomogenziation. Therefore, to make a connection to the continuum picture, we choose the bindingenergies over a representative volume, such that the average H concentration within that volumecorresponds to the expected density of occupied interstitial sites with respect to the bulk H chemicalpotential. The occupation of all interstitial sites within the dislocation line region will be one-half;this choice corresponds to selecting the median value of the binding energy distribution function.We note that, from the results obtained in terms of such comprisingly homogenised models, it is stillpossible to reconstruct the distinct site occupations, but this is restricted to fully relaxed states.
For the parametrisation of grain boundaries, we refer to the results published in [15] for α Fe.They show the dependence of the binding energy of hydrogen at an interstitial site on the spatialdistance to the grain boundary. Precisely, we refer to the calculations for a Σ3 [11̄0](112) grain boundary.The resulting binding energy shows a pronounced attraction with binding energies from 150 to 330 meVin a distance of about 2 Angstroms, while in distances from 2 to 7 Angstroms from the grain boundaryplane, the binding energy ranges from 10 to 40 meV.
4. Results and Discussion
Here, the results of our investigations are presented and it is discussed how they can be interpretedin the context of grain boundary hydrogen embrittlement. On the phenomenological side, our maininterest is in the competition between dislocation and grain boundaries in the aggregation of hydrogen.On the methodological side, the main goal is a quantitative scale transfer from the quantum mechanicaldescription of hydrogen at dislocations and grain boundaries to an elastoplastic deformation model
Metals 2018, 8, 430 9 of 16
on the macroscale that reflects hydrogen aggregation. Apparently, one of the core challenges insuch approaches is the reduction of complexity of the model while still catching the essential effects.We reduce the complexity step by step, which allows us to consider in each stage of simplification theloss of accuracy we inevitably tolerate in the description.
4.1. Modelling Hydrogen Aggregation Considering Dislocation Effects
We aim at the introduction of a composite model for the chemical potential and hydrogenconcentration in the RVEs. This approach introduces an analytic approximation for the non-mechanicalcontributions to the hydrogen chemical potential, leading to a decrease of the computational expenseof the simulations. Therefore, we begin with the comparison of the corresponding analyticalapproximations for the hydrogen distribution in volume elements with and without dislocationsto results from analoguous simulations. These approximations are valid for a single volume element.The most basic approximation excludes also the influence of dislocations, leading to an averageconcentration profile
〈c(µ, E)〉 =exp
(µ−EkBT
)1 + exp
(µ−EkBT
) (15)with an average chemical potential µ = 〈µ〉 and formation energy E = E0 for the bulk description.To include the dependence on the dislocation density in the model, the average concentration is splitinto bulk and dislocation contributions:
〈c〉 = cbulk + νdis (cdis − cbulk) . (16)
Here, νdis is the volume fraction of the dislocation cores and νbulk the volume fraction of the bulk,which are defined as νdis = πr2c ρ and νbulk = 1− νdis, whereby rc describes the radius of the dislocationcore and, therefore, πr2c describes the cross-sectional area of the dislocation line. The system isdescribed in a stationary state ċ = 0, and mechanical contributions are neglected. Equality of thechemical potentials then provides expression for the concentration for the bulk and the dislocationsas cbulk = 〈c(〈µ〉, E0)〉 and cdis = 〈c(〈µ〉, Edis)〉 where we can, based on the calculations in Section 3.3,set Edis = Ēbind.
When comparing the predictions based on the composite analytical model, Equation (15),to the full field simulation results in Figure 5, we see that just the inclusion of the averageddislocation densities is a strict requirement for the accuracy of the approximation. While theperformance of the analytical approximation is convincing when dislocations are included, the situationbecomes much more complex as soon as we introduce grain boundaries in the system to simulatepolycrystalline samples.
Figure 5. Cont.
Metals 2018, 8, 430 10 of 16
Figure 5. Comparison of the numerical solution (blue) with the old analytical solution (red),which includes no dislocation density and the new analytical solution (green) for differentdislocation densities. Including the dislocation density substantially improves the accuracy of theanalytically approximation.
4.2. Modelling Hydrogen Aggregation Considering Dislocation and Grain Boundary Effects
We distinguish two contributions to the hydrogen aggregation at grain boundaries here: on theone side, the stress concentration at the grain boundaries when the system is subjected to mechanicalload and, on the other hand, the binding energies and binding length scales to the grain boundarieswhen the system is free from external stresses. For the latter, we introduce a voxel averaging schemethat allows us to include results from the ab initio calculations that are reported in [15] (see Figure 6).
Figure 6. Illustration of grain boundary and dislocation volume voxel averaging.
Here, Lvoxel is the length of the voxel and lGB the range of attractive sites associated with the grainboundary. Then, the volume fraction of the grain boundary is defined as
νGB =lGB
Lvoxel. (17)
The average hydrogen concentration in this voxel can then be expressed as
〈c〉 = 〈c(〈µ〉, E0)bulk〉+ νdis(〈cdis(〈µ〉, Ebind)〉 − (〈cbulk(〈µ〉, E0)〉
)+ νGB
(〈cGB〉 − 〈cbulk(〈µ〉, E0)〉
). (18)
Metals 2018, 8, 430 11 of 16
Via the ab initio results from [15], the concentration becomes dependent on the distance to thegrain boundary as EGB = EGB(r) when r is the distance from the grain boundary, thus
〈cGB〉 =1
lGB
∫ lGB0〈cGB(r)〉 dr. (19)
However, the grain boundary fraction we introduce via this scheme is then fixed for a givenvoxel length, which leads to undesirable effects. When the voxel length is set to Lvoxel = 1 µm,we obtain a hydrogen concentration profile as shown in Figure 7, corresponding to an estimatedgrain boundary fraction of ∼10−3. This scenario shows basically no remaining hydrogen segregationat the dislocations in the grains. To reduce the grain boundary fraction to values that show lessdominant hydrogen aggregation at the grain boundaries, a voxel length of about 100 micrometres hasto be chosen (see the simulation result obtained for that case in Figure 8). However, in that case, thenumerical parametrisation implies a solution of the elastoplastic equations on an undesirably largespatial scale.
At this point, we have to recognise that defining a representative grain boundary binding energy,which can be used to obtain a composite model, i.e., analytical description, is a rather ineffectiveapproach in comparison to the composite model for the dislocations. The spatial distributionof dislocations can be assumed to suffice the requirements to be fulfilled for a representativevolume element definition, but the distribution of grain boundaries is subject to complex geometricconstraints. Furthermore, the characteristic length scale of the grain boundary distribution is typicallyseveral orders of magnitude larger than the characteristic length scale of the dislocation distribution.This comparably small density requires larger representative volumes for the composite model,which would introduce further inaccuracies to the model.
To reflect the simulation results, we relate them to classical McLean [32] segregation profiles basedon the same ab initio data sets. This includes estimates for the hydrogen segregation from dislocationsto grain boundaries and the effect of hydrogen enrichment at the grain boundaries on segregation tofurther increased concentration levels.
Figure 7. Simulation of a polycrystal containing dislocations with a binding energy to grain boundariesand a voxel size of Lvoxel = 1 µm.
We estimate the influence of a locally hydrogen enriched grain boundary region on the segregationbehaviour of additional hydrogen to those remaining attractive sites at the grain boundary. For thissake, we assume that the work of volume expansion due to the hydrogen is the dominant contributionto the solution energies. Furthermore, we assume that the change in the work of volume expansionunder hydrogen solution with increasing hydrogen content is dominated by the change of the bulkmodulus of the region at the grain boundary.
Metals 2018, 8, 430 12 of 16
Figure 8. Simulation of a polycrystal containing dislocations with a binding energy to grain boundariesand a voxel size of Lvoxel = 100 µm.
Therefore, we consider the following two limiting cases. First, when no other hydrogen atomsare present at the GB, the resulting segregation profile in a simple McLean picture is just based onthe energies reported in [15]. In the second limiting case, we assume that half of all locally available,attractive sites, i.e., with a formation enthalpy ≤ 0.25 eV, are populated. For the Σ3[11̄0](112) bcc grainboundary, this corresponds to a minimum of three hydrogen atoms per volume V ≤ 10−28 m3, which isin the order of 10% at hydrogen at the grain boundary. To estimate the difference in the segregationenergy, assume ∆Eel = ν∆B0 is assumed, with bulk modulus contrast ∆B0 and partial molar volumeof hydrogen ν. The exact elastic grain boundary data we need is not available, but the change of thebulk modulus due to the hydrogen aggregation at the grain boundary is estimated based on the bulkresults reported in [33]. The resulting change ∆B0 is approximated as 15 GPa. For the partial molarvolume of hydrogen, we refer to the comprising studies summarized in [34], which suggest a constantvalue of 1.7 × 10−6 m3/mol of atomic hydrogen (half of a H2 molecule) over wide temperature andpressure ranges. The shift for the segregation energy then amounts to ∆Eel ≈ 15× 1.7× 103/NA eV/J,i.e., ∆Eel ≈ 255 meV.
This value certainly represents a grain boundary that is very densely populated by hydrogen.As the most attractive sites are restricted to a distance of 1–2 Angstroms away from the grain boundary,we assume that the elastic shift of the segregation energies only affects those sites that lie in thisarea. For the Σ3 grain boundary investigated in [15], this corresponds to the four sites withinapprox. 2 Angstroms distance.
The resulting segregation profiles are shown in Figure 9, and the effect of the local elastic softeningon the segregation profile is partially compensated when also dislocations as hydrogen traps are takeninto account. While the detailed data presented in Figure 4 shows a maximal attraction of 0.34 eVin the area close to the dislocation core, we use here the averaged dislocation binding energy of0.14 eV, corrected by an entropic contribution about kBT ln (Vdislocation/Vvoxel). This is consistent as itreproduces an occupation of the dislocation-associated sites, which is reasonable for hydrogen enrichedregions, and we make a similar assumption for the estimate of the occupation shift due to the hydrogeninduced elastic softening. For an interpretation in the context of macroscopic metallurgical processes,a more detailed description of the ambient hydrogen chemical potential is required. Apart from thesurface properties of the samples, especially surface roughness and surface porosity, the humidity ofthe atmosphere is also essential. When the samples are subjected to large thermal gradients due toheat treatment, the distribution of hydrogen at grain boundaries and dislocations close to the surfacewill change depending on the distance to the surface.
Metals 2018, 8, 430 13 of 16
10−9
10−8
10−7
10−6
10−5
10−4
10−3
10−2
10−1
100
0 1 2 3 4 5 6 7
XG
B
Distance to GB (Å)
Figure 9. Segregation profiles for the sites in the vicinity of the grain boundary. The curves withcross symbols correspond to a temperature of 300 K, the curves with box symbols correspond to atemperature of 800 K. For both temperatures, the solid lines correspond to the segregation from a bccbulk site with formation enthalpy ∆E = 0.25 eV to the sites with energies and spatial distance to thegrain boundary plane as reported in [15]. The dashed curves assume that the segregating hydrogenatom moves into a hydrogen enriched region which is limited to those sites within 2 Angstromsdistance to the grain boundary plane. The hydrogen enriched zone has a reduced bulk modulus,and the resulting shift is about 255 meV. The dotted lines correspond to data that takes account thathigh local plasticity densities act as effective traps and that the hydrogen has to overcome the bindingenergy of about 140 meV. We note that the hydrogen is absorbed into the dislocations both for 300 K and800 K from those sites that are more than 2 Angstroms away, expressed by positive segregation energies.This leads to a weak depopulation of this region at 800 K and a pronounced depopulation at 300 K.
This resulting effect of hydrogen binding to dislocations and hydrogen enrichment due to reducedmechanical resistance to hydrogen aggregation is a high local hydrogen density at the grain boundary.Though these results are based on estimates for the bulk modulus contrast and an effective dislocationbinding energy, which result from a site occupation median, they exhibit the weakness of ferritic grainboundaries to hydrogen accumulation. For increasingly high levels of hydrogen aggregation to thegrain boundary, as they are required for hydrogen embrittlement, a kinetic transport of hydrogen isrequired in addition to thermodynamically driven transport. As recently pointed out in [35], hydrogenshielded slip transfer to grain boundaries might offer not only a source for grain boundary stressconcentration, but also this non-thermodynamical hydrogen transport process.
At this point, it is worth discussing the effect of the presence of hydrogen atoms along the grainboundaries on the plastic behavior on the polycrystalline metals. Recent simulations [35] show thathydrogen atoms have multiple effects of the dislocation–GB interactions. First of all, the segregatedhydrogen atoms can develop stress field around the grain boundaries. These stress fields which stemfrom the misfit volumetric strain of the H atoms can attract/repel the dislocations. Thus, the averageslip along the GBs can change [35]. This change promotes the accumulation of slip in local regionsalong the boundary that can lead to the formation of nano-cracks and voids.
Moreover, the presence of H atoms can not only significantly increase the critical shear stressneeded for resolving the lattice dislocation in the grain boundaries, but it can also change the natureof the GB–dislocation interaction. The presence of H atoms can block the dissociation of the lattice
Metals 2018, 8, 430 14 of 16
dislocations into GB-dislocation. Thus, the slip either remains along the grain boundary or is transitedto the adjacent grain at significantly higher stresses. This leads to the formation of more populatedpile-ups and eventually leads to intergranular fracture of the grain boundary surfaces. The dislocationsthat are present in the pile ups can attract hydrogen atoms and deliver it to the grain boundary.As shown in previous studies in nickel, these extra hydrogen atoms can reduce the fracture energysignificantly [36] and make brittle fracture favourable. This intergranular fracture cannot be achievedby considering only the equilibrium segregation hydrogen atoms along the boundary [37]. However,clarification of the kinetic aspects of this process needs further investigation.
5. Conclusions
Within our attempt to find efficient and predictive models for hydrogen segregation basedon ab initio data, we present an analytic composite model for dislocation RVEs. Due to thecomparably homogeneous distribution of dislocations, the length scales of defect separation anddefect extent are unproblematic for the representative volume approach for dislocations and wecan introduce an effective binding energy that leads to good agreement in the efficient compositemodel and full field simulations. When extended to also include grain boundaries in an RVEspirit, also based on ab initio determined binding energies, we recognise a conceptual difficultyof the analytical model. This challenge originates from the strong seperation of the length scalesdescribing defect extent and defect distribution in the case of grain boundaries. A thorough approachto this problem would first demand a comprising analysis of the limitations of scale transfersbetween the description of grain boundaries on the ab initio scale and within the crystal plasticitypicture, which models grain boundaries indirectly. Therefore, one of the key challenges is the vastcombinatorical complexity of compositional and structural degrees of freedom in grain boundaries.On the one hand, the computational expense of state-of-the-art grain boundary calculations, which stillexhibit substantial discrepancies to experimental measurements, is enormous. On the other hand,there are few approximative schemes available to interpolate or extrapolate data sets to differing grainboundaries, even if such data sets are available. Consequently, any comparability to experiments islimited to well defined model systems at the moment.
Apart from this methodological challenge, the simulations and theoretical considerations predicta strong hydrogen segregation in atomic distance from grain boundaries well in competition withdislocation based aggregation when local hydrogen occupation is elevated at the grain boundary.This competition between hydrogen segregation at dislocation and grain boundaries is also observedin the experimental measurements. In the low hydrogen concentration condition, the cleavagefracture indicates weak interaction between diffusive hydrogen and grain boundary, whereas theinteraction becomes intensified with a higher amount of hydrogen. Therefore, there is still a challengeto quantitatively define the critical hydrogen contents leading to grain boundary decohesion fordifferent material groups.
Author Contributions: All authors of the manuscript have contributed to the investigations that produced thepresented results and the writing of the manuscript.
Acknowledgments: This work has been supported by the Collaborative Research Center 761 “Stahl ab initio” ofthe German Research Foundation. The authors gratefully acknowledge the computing time on the supercomputerJURECA at Forschungszentrum Jülich.
Conflicts of Interest: The authors declare no conflict of interest.
References
1. Petch, N.J. The lowering of fracture-stress due to surface adsorption. Philos. Mag. 1956, 1, 331–337. [CrossRef]2. Birnbaum, H.K.; Sofronis, P. Hydrogen-enhanced localized plasticity—A mechanism for hydrogen-related
fracture. Mater. Sci. Eng. A 1994, 176, 191–202. [CrossRef]3. Kirchheim, R. Reducing grain boundary, dislocation line and vacancy formation energies by solute
segregation. I. Theoretical background. Acta Mater. 2007, 55, 5129–5138. [CrossRef]
http://dx.doi.org/10.1080/14786435608238106http://dx.doi.org/10.1016/0921-5093(94)90975-Xhttp://dx.doi.org/10.1016/j.actamat.2007.05.047
Metals 2018, 8, 430 15 of 16
4. Kirchheim, R. Reducing grain boundary, dislocation line and vacancy formation energies by solutesegregation: II. Experimental evidence and consequences. Acta Mater. 2007, 55, 5139–5148. [CrossRef]
5. Lynch, S. Environmentally assisted cracking: Overview of evidence for an adsorption-induced localised-slipprocess. Acta Metall. 1988, 36, 2639–2661. [CrossRef]
6. Nagumo, M. Hydrogen related failure of steels—A new aspect. Mater. Sci. Technol. 2004, 20, 940–950.[CrossRef]
7. Takai, K.; Shoda, H.; Suzuki, H.; Nagumo, M. Lattice defects dominating hydrogen-related failure of metals.Acta Mater. 2008, 56, 5158–5167. [CrossRef]
8. Crabtree, G.W.; Dresselhaus, M.S.; Buchanan, M.V. The hydrogen economy. Phys. Today 2004, 57, 39–44.[CrossRef]
9. Turner, J.A. Sustainable hydrogen production. Science 2004, 305, 972–974. [CrossRef] [PubMed]10. Figueroa, D.; Robinson, M. The effects of sacrificial coatings on hydrogen embrittlement and re-embrittlement
of ultra high strength steels. Corros. Sci. 2008, 50, 1066–1079. [CrossRef]11. Rhodes, P. Environment-assisted cracking of corrosion-resistant alloys in oil and gas production
environments: A review. Corrosion 2001, 57, 923–966. [CrossRef]12. Barrera, O.; Bombac, D.; Chen, Y.; Daff, T.; Galindo-Nava, E.; Gong, P.; Haley, D.; Horton, R.; Katzarov, I.;
Kermode, J.; et al. Understanding and mitigating hydrogen embrittlement of steels: A review of experimental,modelling and design progress from atomistic to continuum. J. Mater. Sci. 2018, 53, 6251–6290. [CrossRef]
13. Jemblie, L.; Olden, V.; Akselsen, O.M. A review of cohesive zone modelling as an approach for numericallyassessing hydrogen embrittlement of steel structures. Philos. Trans. R. Soc. A 2017, 375, 20160411. [CrossRef][PubMed]
14. Koyama, M.; Akiyama, E.; Lee, Y.K.; Raabe, D.; Tsuzaki, K. Overview of hydrogen embrittlement in high-Mnsteels. Int. J. Hydrogen Energy 2017, 42, 12706–12723. [CrossRef]
15. Du, Y.A.; Ismer, L.; Rogal, J.; Hickel, T.; Neugebauer, J.; Drautz, R. First-principles study on the interaction ofH interstitials with grain boundaries in α-and γ-Fe. Phys. Rev. B 2011, 84, 144121. [CrossRef]
16. Troiano, A.R. The role of hydrogen and other interstitials in the mechanical behavior of metals. Trans. ASM1960, 52, 54–80. [CrossRef]
17. Oriani, R. A mechanistic theory of hydrogen embrittlement of steels. Ber. Bunsengesellsch. Phys. Chem. 1972,76, 848–857.
18. Oriani, R.; Josephic, P. Equilibrium aspects of hydrogen-induced cracking of steels. Acta Metall. 1974,22, 1065–1074. [CrossRef]
19. Baechem, C. A New Model for Hydrogen-Assisted Cracking. Met. Trans. 1972, 3, 437–451.20. Von Pezold, J.; Lymperakis, L.; Neugebeauer, J. Hydrogen-enhanced local plasticity at dilute bulk H
concentrations: The role of H–H interactions and the formation of local hydrides. Acta Mater. 2011,59, 2969–2980. [CrossRef]
21. Leyson, G.; Grabowski, B.; Neugebauer, J. Multiscale description of dislocation induced nano-hydrides.Acta Mater. 2015, 89, 50–59. [CrossRef]
22. Roters, F.; Eisenlohr, P.; Kords, C.; Tjahjanto, D.; Diehl, M.; Raabe, D. DAMASK: The Duesseldorf AdvancedMaterial Simulation Kit for studying crystal plasticity using an FE based or a spectral numerical solver.Procedia IUTAM 2012, 3, 3–10. [CrossRef]
23. Hirth, J. Effects of hydrogen on the properties of iron and steel. Metall. Trans. A 1980, 11, 861–890. [CrossRef]24. Shanthraj, P.; Sharma, L.; Svendsen, B.; Roters, F.; Raabe, D. A phase field model for damage in
elasto-viscoplastic materials. Comput. Methods Appl. Mech. Eng. 2016, 312, 167–185. [CrossRef]25. Nemat-Nasser, S.; Hori, M. Micromechanics: Overall Properties of Heterogenous Materials; Elsevier
North-Holland: Amsterdam, The Netherlands, 1999.26. Peirce, D.; Asaro, R.; Needleman, A. Material rate dependence and localized deformation in crystalline
solids. Acta Metall. 1983, 31, 1951–1976. [CrossRef]27. Roters, F.; Eisenlohr, P.; Hantcherli, L.; Tjahjanto, D.; Bieler, T.; Raabe, D. Overview of constitutive laws,
kinematics, homogenization and multiscale methods in crystal plasticity finite-element modeling: Theory,experiments, applications. Acta Mater. 2010, 58, 1152–1211. [CrossRef]
28. Cahn, J.W.; Hilliard, J.E. Free energy of a nonuniform system. I. Interfacial free energy. J. Chem. Phys. 1958,28, 258–267. [CrossRef]
http://dx.doi.org/10.1016/j.actamat.2007.05.033http://dx.doi.org/10.1016/0001-6160(88)90113-7http://dx.doi.org/10.1179/026708304225019687http://dx.doi.org/10.1016/j.actamat.2008.06.031http://dx.doi.org/10.1063/1.1878333http://dx.doi.org/10.1126/science.1103197http://www.ncbi.nlm.nih.gov/pubmed/15310892http://dx.doi.org/10.1016/j.corsci.2007.11.023http://dx.doi.org/10.5006/1.3290320http://dx.doi.org/10.1007/s10853-017-1978-5http://dx.doi.org/10.1098/rsta.2016.0411http://www.ncbi.nlm.nih.gov/pubmed/28607190http://dx.doi.org/10.1016/j.ijhydene.2017.02.214http://dx.doi.org/10.1103/PhysRevB.84.144121http://dx.doi.org/10.1007/s13632-016-0319-4http://dx.doi.org/10.1016/0001-6160(74)90061-3http://dx.doi.org/10.1016/j.actamat.2011.01.037http://dx.doi.org/10.1016/j.actamat.2015.01.057http://dx.doi.org/10.1016/j.piutam.2012.03.001http://dx.doi.org/10.1007/BF02654700http://dx.doi.org/10.1016/j.cma.2016.05.006http://dx.doi.org/10.1016/0001-6160(83)90014-7http://dx.doi.org/10.1016/j.actamat.2009.10.058http://dx.doi.org/10.1063/1.1744102
Metals 2018, 8, 430 16 of 16
29. McEniry, E.J.; Drautz, R.; Madsen, G. Environmental tight-binding modeling of nickel and cobalt clusters.J. Phys. Condens. Matter 2013, 25, 115502. [CrossRef] [PubMed]
30. McEniry, E.J.; Hickel, T.; Neugebauer, J. Hydrogen behaviour at twist {110} grain boundaries in α-Fe.Philos. Trans. A 2017, 375, 20160402. [CrossRef] [PubMed]
31. Clouet, E.; Ventelon, L.; Willaime, F. Dislocation core field. II. Screw dislocation in iron. Phys. Rev. B 2011,84, 224107. [CrossRef]
32. Lejcek, P. Grain Boundary Segregation in Metals; Springer: Berlin, Germany, 2010.33. Psiachos, D.; Hammerschmidt, T.; Drautz, R. Ab initio study of the modification of elastic properties of
alpha-iron by hydrostatic strain and by hydrogen interstitials. Acta Mater. 2011, 59, 4255–4263. [CrossRef]34. Peisl, H. Topics in Applied Physics: Hydrogen in Metals I; Springer: Berlin, Germany, 1978.35. Tehranchi, A. Atomistic Mechanisms of Hydrogen Embrittlement; EPFL: Lausanne, Switzerland, 2017; p. 165.36. Tehranchi, A.; Curtin, W. Atomistic study of hydrogen embrittlement of grain boundaries in nickel:
II. Decohesion. Model. Simul. Mater. Sci. Eng. 2017, 25, 075013. [CrossRef]37. Tehranchi, A.; Curtin, W. Atomistic study of hydrogen embrittlement of grain boundaries in nickel:
I. Fracture. J. Mech. Phys. Solids 2017, 101, 150–165. [CrossRef]
c© 2018 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open accessarticle distributed under the terms and conditions of the Creative Commons Attribution(CC BY) license (http://creativecommons.org/licenses/by/4.0/).
http://dx.doi.org/10.1088/0953-8984/25/11/115502http://www.ncbi.nlm.nih.gov/pubmed/23406579http://dx.doi.org/10.1098/rsta.2016.0402http://www.ncbi.nlm.nih.gov/pubmed/28607182http://dx.doi.org/10.1103/PhysRevB.84.224107http://dx.doi.org/10.1016/j.actamat.2011.03.041http://dx.doi.org/10.1088/1361-651X/aa87a6http://dx.doi.org/10.1016/j.jmps.2017.01.020http://creativecommons.org/http://creativecommons.org/licenses/by/4.0/.
IntroductionExperimental FindingsModel FormulationContinuum Model FormulationNumerical Implementation of the Continuum ModelAtomistic Parameterisation
Results and DiscussionModelling Hydrogen Aggregation Considering Dislocation EffectsModelling Hydrogen Aggregation Considering Dislocation and Grain Boundary Effects
ConclusionsReferences